the consolidation of flaking gouache on japanese · pdf filethe consolidation of flaking...
Click here to load reader
Post on 15-Sep-2018
Embed Size (px)
The Consolidation of Flaking Gouache on Japanese Paper
by ALAIN ROCHE & LUCILE DESSENNES
The consolidation of flaking gouache on Japanese paper
Some gouache works, made in the 1930s by Claude Autant-Lara, were damaged in die paint layer.
Extensive areas of gouache including areas of overlapping layers of paint were very cracked. Some
of these were even flaking. In order to select the appropriate treatment, we compared the properties
of five different strengthening agents, prepared to the same concentration (l/o) or same viscosity (3
cp), resp. Samples of gouache, as close as possible to the work of art were prepared, submitted to
accelerated ageing and then consolidated with the strengthening agents: gelatine, sturgeon glue,
polyvinyl alcohol, methylhydroxyethylcellulose and Paraloid B72. Adhesive and cohesive strength
were measured using a peeling test and a shearing test in a traction machine. The different kinds of
break and their areas were studied in order to evaluate the particularities of each product and the
best one for the case in question.
La consolidation de gouaches cailles sur papier Japon
Des gouaches ralises par Claude Autant-Lara au cours des annes 1930 prsentaient plusieurs
types de dgradation. De grandes couches de gouache, quelquefois superposes les unes aux autres,
taient trs craqueles et certaines mme cailles. Afin de trouver une mthode de traitement
approprie nous avons compar les proprits de cinq agents consolidant diffrents prpares
respectivement au mme taux de concentration (1%) et de viscosit (3cp). Des chantillons de
gouache se rapprochant le plus possible du cas tudie ont t prpares, soumis au vieillissement
artificiel, puis consolides au moyen des agents suivants : glatine, colle d'esturgeon, alcool
polyvinylique, mthylcellulose et Paraloid B72. Les forces d'adhsion et de cohsion ont t
tudies a 1'aide d'un test de pelage et d'un test de cisaillement par un appareil de mesure de
rsistance a la traction. Ensuite la nature des ruptures et les diffrents endroits ou elles se sont
produites ont t tudies afin d'valuer les particularits de chaque agent consolidant et de
slectionner celui qui est le mieux approprie au cas tudie.
Die Festigung van abblatternder Gouache aufjapanpapier
Einige Gouache-Blatter aus den 30er Jahren des 20. Jh. von Claude Autant-Lara wiesen schwere
Schaden auf. Weite Bereiche, deren Farbschichten teilweise ubereinander lagen, zeigten Craquele,
einige schuppenformige Abhebungen. Um eine geeignete Behandlungsmethode zu finden, wur-den
funf verschiedene Festigungsmittel getestet: Gelatine, Hausenblase, Polyvinylalkohol, Methyl-
cellulose und Paraloid B72. Sie wurden in gleicher Konzentration (1%) bzw. in gleicher Viskosi-tat
(3 cp) zubereitet. Sodann wurden Muster hergestellt, die in Material und Aufbau den zur Rede
stehenden Kunstwerken moglichst nahe kamen, und mil den genannten Festigungsmitteln
behandelt. Mit Hilfe eines Zugfestigkeitspriifgerats wurden in einem Abschal-, und in einem
Schertest Adhasion und Kohasion gemessen. Danach wurden Art und Bereich der auftrtetenden
Briiche untersucht, um die spezifische Wirkung der Festigungsmittel zu erfassen.
We had to consolidate five gouache studies for scenery, made by Claude Autant-Lara around 1937.
All were very cracked, although only one painting was flaking. The gouache used was made out of
gum arabic, according to a traditional recipe. The gouache was thick and layered in places. It was
painted on a Japanese paper called "Imperial japon", made out of eastern mitsumata fibers. The
spatial density of the cracks was variable, depending on the paint colour, its thickness, and whether
it had been applied onto another layer. We noticed that the red colour and its variants, purple and
orange, were always cracked. On the other hand, the white and mixtures containing it, never
cracked. It appeared that cracking was most evident in the areas where gouache had been applied
thickly and particularly where there were multiple layers of paint. Flaking was due to both a loss of
cohesion within the colour (cracks), and a loss of adhesion between the paint layer and the paper
The formation of the cracks was caused by several factors. Gouache is water-based consisting of a
pigment, a mineral charge (calcium carbonate), a binding agent (traditionally gum arable) and
water, primarily the solvent for the binding agent and partly remaining in the paint layer as a
plasticizer. The water particles are bound to the hydrophilic gum arabic particles, allowing them to
slide and make the paint layer flexible. However, water evaporates; which is why water-retaining
substances such as honey or, more recently, glycerol1, were added to gouache. In the case reported
here, the paint seems to have been quite thick, which gives intensity to the colour, but also means
there is a tendency for the paint to become brittle. Moreover, the thicker the paint layer, the stronger
the internal tensions during drying. While a thin layer of gouache dries quickly and evenly, the top
area of a thick layer dries more quickly than the material beneath. Very often, the tensions between
layers result in concave2 concentrating humidity. The surface tension and the forces within the paint
layer work in the same direction, i.e. parallel, but not in equal amounts, which results in cupping1.
Quite often cracks, which appear during ageing, are due to the loss in elasticity of the binding agent.
Indeed, gum arabic loses water in the course of ageing. Hydrolysis and the photo-oxidation of its
glucosidic molecules results in chain scission, which leads to the production of glucose units.
Cupping can become deeper with time, lift from the support, and form flakes by absorbing and
desorbing free water from the atmosphere. As soon as cracks appear, water is no longer distributed
evenly through the entire paint layer, it flows more easily through cracks4 causing variation in
tension in the cracked areas.
Consolidation of flaking gouache can be achieved by regeneration of the binding agent or by adding
a strengthening agent. The former can be achieved by humidifying in a water saturated atmosphere.
However, this is not a real regeneration. Indeed, a fraction of the water contained in a non-altered
paint layer is chemically bound to the gum arabic. Thus, desiccation associated with natural ageing
is an irreversible chemical phenomenon. However, humidification can ease the application of a
strengthening agent. It may indeed soften the cupped areas, so that they can be flattened with light
pressure. The other alternative, the addition of a strengthening agent into the paint layer, can be
seen as being problematic because it is practically irreversible.
Gouache consolidation aims at strengthening the cohesion of the paint layer and its adhesion to the
paper support. Two qualities of the agent in liquid form are of crucial importance: surface tension
and viscosity. Both influence the way it penetrates into the paint layer.
Comprehensive studies were necessary to select a good strengthening agent. Indeed, in
consolidating the large painted areas we had to find something chemically and physically stable, as
well as aesthetically neutral. Samples, or dummies of the paints in question were made, using
materials as close as possible to those used by the artist. After artificial ageing, the samples were
consolidated with several different concentrations of dissolved agents. After drying, a peeling and a
shearing test were performed.
THE STRENGTHENING AGENTS
We tested three different types of agent:
Two natural products: gelatine and sturgeon glue1. They are both traditionally used in the
consolidation of flaking gouache.
Two synthetic water-soluble polymers: a methylhydroxyethylcellulose (Tylose MH 300,
Hoechst), and a polyvinyl alcohol (Rhodoviol 4/125, Hoechst). The first has a good adhesive power
and a high viscosity even at low concentrations. The other is used as a modern binding agent for
watercolour and in the paper industry for coating6.
A synthetic solvent soluble polymer: Paraloid B72 (Rohm & Haas), dissolved in 40% toluene
and 60% ethanol. It is one of the most commonly used resins in conservation. However, secondary
effects have been observed when applied to paper'.
Two solutions were prepared for each of these compounds. The first was a 1% solution, which is
the maximum concentration used for aqueous strengthening agents. Indeed, if used at a higher
concentration, the product would start to be noticeable and make the gouache brighter. Note that the
viscosity of the 1% solutions varied with the different substances (Table 1).
The second solution was prepared so that its viscosity was 3 cP. This corresponded to the minimum
concentration for the consolidation of flaking pigment on paper using poly vinyl alcohol and
Paraloid B72. For the other, more viscous adhesives, the concentration resulting in 3 cP viscosity
was different: 1% for gelatine and less than 0.5% for methylhydroxyethylcellulose (Table 2). For
sturgeon glue, this viscosity could not be achieved: 1% concentration resulted in 1.5 cP viscosity,
any higher was already in a gel.
Table 1: Viscosity (cP